- Nano Express
- Open Access
Fabrication of ultrahigh-density nanowires by electrochemical nanolithography
© Chen et al; licensee Springer. 2011
- Received: 28 March 2011
- Accepted: 11 July 2011
- Published: 11 July 2011
An approach has been developed to produce silver nanoparticles (AgNPs) rapidly on semiconductor wafers using electrochemical deposition. The closely packed AgNPs have a density of up to 1.4 × 1011 cm-2 with good size uniformity. AgNPs retain their shape and position on the substrate when used as nanomasks for producing ultrahigh-density vertical nanowire arrays with controllable size, making it a one-step nanolithography technique. We demonstrate this method on Si/SiGe multilayer superlattices using electrochemical nanopatterning and plasma etching to obtain high-density Si/SiGe multilayer superlattice nanowires.
- Immersion Time
- Pulse Length
- Nanowire Array
- Plasma Etching
- SiGe Layer
Low-dimensional systems are of high interest because their unique properties can improve device performance in a range of applications, including optics [1, 2], mechanics , microelectronics , and magnetics . These systems have enhanced surface and quantum confinement effects caused by the large surface-to-volume ratio and small size, making them dramatically different from their bulk counterparts. Superlattice nanowires have the potential to improve the performance of thermoelectronics [6–9], small sizes have lower thermal conductivity [8, 9], and they can be made at a high density, thus providing improved performance.
Generally, there are two major approaches in the fabrication of nanostructures: bottom-up  and top-down . Among the various bottom-up methods, vapor-liquid-solid (VLS) growth is one of the most popular and is used to grow nanostructures such as nanowires [12–14]. VLS growth uses a catalytic liquid-alloy phase that can rapidly adsorb a vapor to supersaturation levels, in which crystal growth can subsequently occur from nucleated seeds at the liquid-solid interface. It is a relatively simple method and yields a large quantity of nanowires from a single growth. However, the requirement of metal particle catalysts risks contaminating the nanowires , and it is not easy to control the density and nanowire size, shape, and crystal orientation simultaneously . Additionally, twin boundaries normally form in the VLS growth, which may affect the subsequent nanowire performance .
Typically, top-down approaches involve lithography, which defines the lateral size and shape of the final structure using an electron/photon-sensitive resist as mask material. Examples are electron beam lithography  and X-ray nanolithography . For example, Zhong et al. have reported ordered SiGe/Si superlattice pillars combining holographic lithography, molecular beam epitaxy (MBE) growth, and wet chemical etching . Although e-beam and X-ray lithographies create uniformly distributed and ordered templates for further top-down processing, they are expensive and time consuming. They also require several processing steps, involving photoresist deposition/removal and chemical or ion beam etching. Other approaches utilize self-assembling  structures such as block copolymers  or anodic aluminum oxide as masks [13, 23]. The outputs of self-assembling techniques are uniform in size and ordered over a large scale; however, they usually require additional deposition, baking, etching, and stripping processes.
Instead of a patterned photoresist, it is also possible to use nanoparticles (NPs) as a nanolithography mask. NPs can be prepared by electrochemical deposition (ECD), an easy, fast, economical, and straightforward way to deposit materials directly on top of semiconductors  or metals [25–27]. To the best of our knowledge, ECD of NPs has not been reported in top-down semiconductor nanostructure fabrication.
We deposit silver nanoparticles (AgNPs) in sizes of tens of nanometers, using pulsed-current driven ECD. By adjusting the deposition conditions, we achieve high-density AgNPs with uniform size and spacing. The resulting one-step electrochemically deposited AgNPs are very robust and can survive further processing. Therefore, they can be used as a hard mask for plasma etching or as a metal-assisted etching mask . By using this mask in combination with chemical vapor deposition (CVD) growth and plasma etching, we are able to fabricate ultrahigh-density (6.2 × 1010 cm-2) Si/SiGe superlattice nanowire arrays over a large area, with individual wires < 30 nm in diameter and approximately 200 nm in length.
The Si/SiGe superlattice wafer is prepared using low-pressure CVD. We grow a ten-period Si/Si0.82Ge0.18 superlattice structure on Si wafers (Si(001), p-type, nominal doping density of 1015 cm-3), and cap the superlattice with Si (Figure 1b). The layer thickness is 10.8 nm for Si and 7.0 nm for the SiGe alloy, as confirmed by X-ray diffraction (XRD, PANalytical X'Pert MRD, PANalytical, Inc., Westborough, MA, USA). Both layers are grown at 580°C, with silane and germane as precursors. The root mean square surface roughness measured by atomic force microscopy (AFM Digital Instrument Nanoscope IV, Veeco Instruments, Santa Barbara, CA, USA) after CVD growth of all the layers is 0.7 nm.
Before performing ECD, we dip the as-grown superlattice wafer in hydrofluoric acid to remove the native oxide on the top Si layer. After rinsing in deionized water (DI) for 5 min, we quickly immerse it into the AgNO3 solution (1 × 10-4 M).
We use pulsed current as the deposition driving force to deposit nanoparticles because this approach is very controllable when depositing a small amount of material. The pulsed signal consists of a long period (T) with a short pulse length (τ). Various immersion times (t) and pulse lengths (τ = 1 ms to 0.5 s) were tried in the experiment in order to obtain AgNPs with uniform small size and high density.
After AgNP deposition, plasma etching is performed to produce superlattice nanowires. The substrate, with the AgNPs acting as a hard mask, is etched by a high-density helicon plasma tool equipped with a diode laser interferometer for in situ etch depth measurement (Figure 1d) . A gas mixture of SF6/C2H2F4 is used. Source power and bias voltage are finely tuned to obtain a vertical etch profile. Using this system, we are able to etch out nanowires up to several microns in length .
For a much shorter pulse length, τ = 1 ms, the general trend of size distribution is the same, but particles are much smaller and the uniform size distribution lasts to longer immersion times. For comparison, the results of the 50-s immersion time are shown in Figure 2f.
The applied electric field is the driving force of the Ag+ reduction reaction. Each positive pulse applied on the electrode drives Ag+ ions towards the cathode, here the Si surface. The pulse length of the pulse determines the number of adatoms arriving on the surface. Because the applied voltage (20 V) is much higher than the overpotential (300 mV), the effects of the space charge layer and the Helmholtz layer can be ignored when considering the potential profile across the substrate/solution interface .
Low ion concentration or long immersion time can cause a transition from weak interparticle interaction to strong interaction. At long immersion times (t > 40 s in our experiment), depletion layers at adjacent particles merge to create an approximately planar diffusion layer across the entire surface (Figure 3b); this strong interparticle interaction makes the flux of ions per unit area on the surface more uniform. Because the nucleation density is locally variable, densely nucleated regions are therefore expected to have a slower growth rate than regions of the same size but encompassing a smaller number of nanoparticles. Thus, when the immersion time reaches 50 s the size distribution becomes less uniform (Figure 2e). At the same time, Ostwald ripening decreases particle size uniformity as smaller islands are eliminated by the larger ones .
By reducing the pulse length, we achieve higher particle density and smaller particle size while still maintaining good size uniformity. In Figure 2f, the AgNPs have a density of 1.4 × 1011 cm-2, which is almost twice the density for τ = 0.5 s (Figure 2e), while the relative standard deviation of size is only 42%.
where n/s 0 is the particle density on the SEM image area.
Using high-resolution transmission electron microscopy (HRTEM, Philips, CM200UT, Philips Electron Optics BV, Eindhoven, The Netherlands), we can explore the layered structure of the nanowires. Figure 5c, a relatively low-magnification image, shows the periodic variation in brightness representative of the layers. The darker regions are the SiGe alloy because Ge scatters electrons more strongly. We can clearly see the interfaces between Si and SiGe layers. Figure 5d demonstrates that the nanowires are single crystals, as we expect from the MBE growth. In the VLS growth of nanowires, normally twin boundaries are observed . With our method, this problem is eliminated because the starting material is a CVD-grown single-crystalline 2D superlattice.
The SiGe alloy etches faster than pure Si in a SF6/C2H2F4 plasma, giving the edge of the wire a scalloped appearance, effectively introducing surface roughness to the sidewall. The etching process does not affect the crystallographic properties of the superlattice. The surface roughness may result in enhanced phonon scattering .
Si and Ge nanowires have been considered as potentially good thermoelectric materials, because of the reduced thermal conductivity at small dimensions. Superlattice nanowires have even greater potential because of the band offset between Si and SiGe . Thus, electric conductivity is possibly improved through the superlattice structure [38, 39]. The combination of excellent superlattice with edge roughness of our etched nanowires may therefore bring higher thermoelectric efficiency for group IV materials than has been possible so far.
In this paper, we introduce a one-step nanolithography method to fabricate quantum wires with diameters down to 15 nm using electrochemically deposited AgNPs. The AgNP density obtained is as high as 1.4 × 1011 cm-2 with coverage up to 37% over a large area. By adjusting the pulse length and immersion time, the size and density of AgNPs can be well controlled. We demonstrate that these high-density AgNPs can be used as a hard etching mask to fabricate vertically aligned Si/SiGe superlattice nanowires. Because the method does not need lithography to define the pattern, it is much less expensive and can make very small patterns that may have considerable use even if the pattern is not totally uniform. The size and coverage of etched nanostructures only depend on the AgNPs. The method can be used with substrates of any material as long as it conducts sufficiently to form a cathode for the electrochemical process, and a proper etch chemistry to which Ag is resistant is available. The AgNP mask can be used in both metal-assisted etching to etch Si and SiGe and RIE to etch most other semiconductor materials. The method has the potential to make nanowires of different materials, as well as different orientations. It should be very useful in making devices requiring nanowires, such as nanothermoelectronic devices, that require a small size, narrow dispersion, and high density.
We are grateful to F. Flack for reading the manuscript. This research was supported by DOE-BES, grant no. DE-FG02-03ER46028, except as detailed below. FC was partially supported by the Chinese Scholarship Council (CSC). AMK was supported by a SMART Fellowship. Etching (YHT and EAW) was supported by NSF/MRSEC, grant no. DMR-0520527. Facilities support from NSF/MRSEC is acknowledged.
- Jacobsen RS, Andersen KN, Borel PI, Fage-Pedersen J, Frandsen LH, Hansen O, Kristensen M, Lavrinenko AV, Moulin G, Ou H, Peucheret C, Zsigri B, Bjarklev A: Strained silicon as a new electro-optic material. Nature 2006, 441: 199–202. 10.1038/nature04706View ArticleGoogle Scholar
- Feng P, Mönch I, Huang G, Harazim S, Smith EJ, Mei Y, Schmidt OG: Local-illuminated ultrathin silicon nanomembranes with photovoltaic effect and negative transconductance. Adv Mater 2010, 22: 3667–3671. 10.1002/adma.201000583View ArticleGoogle Scholar
- Heidelberg A, Ngo LT, Wu B, Phillips MA, Sharma S, Kamins TI, Sader JE, Boland JJ: A generalized description of the elastic properties of nanowires. Nano Lett 2006, 6: 1101–1106. 10.1021/nl060028uView ArticleGoogle Scholar
- Liu AS, Jones R, Liao L, Samara-Rubio D, Rubin D, Cohen O, Nicolaescu R, Paniccia M: A high-speed silicon optical modulator based on a metal-oxide-semiconductor capacitor. Nature 2004, 427: 615–618. 10.1038/nature02310View ArticleGoogle Scholar
- Nielsch K, Wehrspohn RB, Barthel J, Kirschner J, Gösele U, Fischer SF, Kronmuller H: Hexagonally ordered 100 nm period nickel nanowire arrays. Appl Phys Lett 2001, 79: 1360–1362. 10.1063/1.1399006View ArticleGoogle Scholar
- Harman TC, Taylor PJ, Walsh MP, LaForge BE: Quantum dot superlattice thermoelectric materials and devices. Science 2002, 297: 2229–2232. 10.1126/science.1072886View ArticleGoogle Scholar
- Venkatasubramanian R, Siivola E, Colpitts T, O'Quinn B: Thin-film thermoelectric devices with high room-temperature figures of merit. Nature 2001, 413: 597–602. 10.1038/35098012View ArticleGoogle Scholar
- Li D, Wu Y, Kim P, Shi L, Yang P, Majumdar A: Thermal conductivity of individual silicon nanowires. Appl Phys Lett 2003, 83: 2934–2936. 10.1063/1.1616981View ArticleGoogle Scholar
- Li DY, Wu Y, Fan R, Yang PD, Majumdar A: Thermal conductivity of Si/SiGe superlattice nanowires. Appl Phys Lett 2003, 83: 3186–3188. 10.1063/1.1619221View ArticleGoogle Scholar
- Geissler M, Xia Y: Patterning: principles and some new developments. Adv Mater 2004, 16: 1249–1269. 10.1002/adma.200400835View ArticleGoogle Scholar
- Huang Y, Duan X, Cui Y, Lauhon LJ, Kim KH, Lieber CM: Logic gates and computation from assembled nanowire building blocks. Science 2001, 294: 1313–1317. 10.1126/science.1066192View ArticleGoogle Scholar
- Wacaser BA, Dick KA, Johansson J, Borgstrom MT, Deppert K, Samuelson L: Preferential interface nucleation: an expansion of the VLS growth mechanism for nanowires. Adv Mater 2009, 21: 153–165. 10.1002/adma.200800440View ArticleGoogle Scholar
- Wang XD, Summers CJ, Wang ZL: Large-scale hexagonal-patterned growth of aligned ZnO nanorods for nano-optoelectronics and nanosensor arrays. Nano Lett 2004, 4: 423–426. 10.1021/nl035102cView ArticleGoogle Scholar
- O'Toole M, Boland JJ: A solid-liquid-vapor mechanism for anisotropic silicon etching. Appl Phys Lett 2008, 93: 263107–1-3. 10.1063/1.3055606View ArticleGoogle Scholar
- Wang N, Tang YH, Zhang YF, Lee CS, Bello I, Lee ST: Si nanowires grown from silicon oxide. Chem Phys Lett 1999, 299: 237–242. 10.1016/S0009-2614(98)01228-7View ArticleGoogle Scholar
- Johansson J, Karlsson LS, Dick KA, Bolinsson J, Wacaser BA, Deppert K, Samuelson L: Effects of growth conditions on the crystal structure of gold-seeded gap nanowires. J Cryst Growth 2008, 310: 5102–5105. 10.1016/j.jcrysgro.2008.08.003View ArticleGoogle Scholar
- Morales AM, Lieber CM: A laser ablation method for the synthesis of crystalline semiconductor nanowires. Science 1998, 279: 208–211. 10.1126/science.279.5348.208View ArticleGoogle Scholar
- Mendes PM, Jacke S, Critchley K, Plaza J, Chen Y, Nikitin K, Palmer RE, Preece JA, Evans SD, Fitzmaurice D: Gold nanoparticle patterning of silicon wafers using chemical e-beam lithography. Langmuir 2004, 20: 3766–3768. 10.1021/la049803gView ArticleGoogle Scholar
- Falcaro P, Costacurta S, Malfatti L, Takahashi M, Kidchob T, Casula MF, Piccinini M, Marcelli A, Marmiroli B, Amenitsch H, Schiavuta P, Innocenzi P: Fabrication of mesoporous functionalized arrays by integrating deep x-ray lithography with dip-pen writing. Adv Mater 2008, 20: 1864–1869. 10.1002/adma.200702795View ArticleGoogle Scholar
- Zhong Z, Katsaros G, Stoffel M, Costantini G, Kern K, Schmidt OG, Jin-Phillipp NY, Bauer G: Periodic pillar structures by Si etching of multilayer GeSi/Si islands. Appl Phys Lett 2005, 87: 263102–1-3. 10.1063/1.2150278View ArticleGoogle Scholar
- Wang LJ, Krapek V, Ding F, Horton F, Schliwa A, Bimberg D, Rastelli A, Schmidt OG: Self-assembled quantum dots with tunable thickness of the wetting layer: role of vertical confinement on interlevel spacing. Phys Rev B 2009, 80: 085301–1-9.View ArticleGoogle Scholar
- Mahmoud MA, Tabor CE, El-Sayed MA: Surface-enhanced Raman scattering enhancement by aggregated silver nanocube monolayers assembled by the Langmuir-Blodgett technique at different surface pressures. J Phys Chem C 2009, 113: 5493–5501. 10.1021/jp900648rView ArticleGoogle Scholar
- Geyer N, Huang Z, Fuhrmann B, Grimm S, Reiche M, Nguyen-Duc T-K, de Boor J, Leipner HS, Werner P, Gösele U: Sub-20 nm Si/Ge superlattice nanowires by metal-assisted etching. Nano Lett 2009, 9: 3106–3110. 10.1021/nl900751gView ArticleGoogle Scholar
- Vereecken PM, Strubbe K, Gomes WP: An improved procedure for the processing of chronoamperometric data: application to the electrodeposition of Cu upon (100) n-GaAs. J Electroanal Chem 1997, 433: 19–31. 10.1016/S0022-0728(97)00195-2View ArticleGoogle Scholar
- Manne S, Hansma PK, Massie J, Elings VB, Gewirth AA: Atomic-resolution electrochemistry with the atomic force microscope-copper deposition on gold. Science 1991, 251: 183–186. 10.1126/science.251.4990.183View ArticleGoogle Scholar
- Gao X, Hamelin A, Weaver MJ: Potential-dependent reconstruction at ordered Au(100)-aqueous interfaces as probed by atomic-resolution scanning tunneling microscopy. Phys Rev Lett 1991, 67: 618–621. 10.1103/PhysRevLett.67.618View ArticleGoogle Scholar
- Sonnenfeld R, Schardt BC: Tunneling microscopy in an electrochemical-cell-images of Ag plating. Appl Phys Lett 1986, 49: 1172–1174. 10.1063/1.97405View ArticleGoogle Scholar
- Ting YH, Park SM, Liu CC, Liu XS, Himpsel FJ, Nealey PF, Wendt AE: Plasma etch removal of poly(methyl methacrylate) in block copolymer lithography. J Vac Sci Technol B 2008, 26: 1684–1689. 10.1116/1.2966433View ArticleGoogle Scholar
- Mizuhata M, Miyake T, Nomoto Y, Deki S: Deep reactive ion etching (deep-RIE) process for fabrication of ordered structural metal oxide thin films by the liquid phase infiltration method. Microelectron Eng 2008, 85: 355–364. 10.1016/j.mee.2007.07.006View ArticleGoogle Scholar
- Oskam G, Long JG, Natarajan A, Searson PC: Electrochemical deposition of metals onto silicon. J Phys D-Appl Phys 1998, 31: 1927–1949. 10.1088/0022-3727/31/16/001View ArticleGoogle Scholar
- Stiger RM, Gorer S, Craft B, Penner RM: Investigations of electrochemical silver nanocrystal growth on hydrogen-terminated silicon(100). Langmuir 1999, 15: 790–798. 10.1021/la980800bView ArticleGoogle Scholar
- Fransaer JL, Penner RM: Brownian dynamics simulation of the growth of metal nanocrystal ensembles on electrode surfaces from solution. I. Instantaneous nucleation and diffusion-controlled growth. J Phys Chem B 1999, 103: 7643–7653. 10.1021/jp990622aView ArticleGoogle Scholar
- Ratke L, Voorhees PW: Growth and coarsening: Ostwald ripening in material processing. New York: Springer; 2002.View ArticleGoogle Scholar
- Rhee H, Lee HM, Namkoung YM, Kim CK, Chae H, Kim YW: Dependence of etch rates of silicon substrates on the use of C 4 F 8 and C 4 F 6 plasmas in the deposition step of the Bosch process. J Vac Sci Technol B 2009, 27: 33–40. 10.1116/1.3039690View ArticleGoogle Scholar
- Kawata H, Yasuda M, Hirai Y: Si etching with high aspect ratio and smooth side profile for mold fabrication. Jpn J Appl Phys 2006, 45: 5597–5601. 10.1143/JJAP.45.5597View ArticleGoogle Scholar
- Zhang YF, Huang HC: Twin Cu nanowires using energetic beams. Appl Phys Lett 2009, 95: 111914–1-3. 10.1063/1.3232240View ArticleGoogle Scholar
- Chen R, Hochbaum AI, Murphy P, Moore J, Yang PD, Majumdar A: Thermal conductance of thin silicon nanowires. Phys Rev Lett 2008, 101: 105501–1-4.View ArticleGoogle Scholar
- Lin Y-M, Dresselhaus MS: Thermoelectric properties of superlattice nanowires. Phys Rev B 2003, 68: 075304–1-14.View ArticleGoogle Scholar
- Huang MH, Ritz CS, Novakovic B, Yu DC, Zhang Y, Flack F, Savage DE, Evans PG, Knezevic I, Liu F, Lagally MG: Mechano-electronic superlattices in silicon nanoribbons. ACS Nano 2009, 3: 721–727. 10.1021/nn8008883View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.